TIG welding aluminum with square wave alternating current differs from conventional balanced wave TIG welding in the type of wave form used. With a square wave, the time of current flow in either direction is adjustable from 20 to 1. In square wave gas tungsten arc welding, there are the advantages of surface cleaning produced by positive ionic bombardment during the reversed polarity cycle, along with greater weld depth to width ratio produced by the straight polarity cycle. Sufficient aluminum surface cleaning action has been obtained with a setting of approximately 10 percent dcrp. Penetration equal to regular dcsp welding can be obtained with 90 percent dcsp current.
TIG Welding Aluminum with Square Wave Alternating Current Technique
It is necessary to have either superimposed high frequency or high open circuit voltage, because the arc is extinguished every half cycle as the current decays toward zero, and must be restarted each tire. Precision shaped thoriated tungsten electrodes should be used with this process. Argon, helium, or a combination of the two should be used as shielding gas, depending on the application to be used.
TIG Welding Aluminum with Alternating Square Wave Current Joint design
Square wave alternating current welding offers substantial savings over conventional alternating current balanced wave gas tungsten arc welding in weld joint preparation. Smaller V grooves, U grooves, and a thicker root face can be used. A greater depth to width weld ratio is conducive to less weldment distortion, along with favorable welding residual stress distribution and less use of filler wire. With Some slight modification, the same joint designs can be used as in dcsp gas tungsten-arc welding (fig. 7-11).
Subscribe via RSS